Facile Preparation of a Platinum Silicide Nanoparticle-Modified Tip Apex for Scanning Kelvin Probe Microscopy
© Lin et al. 2015
Received: 24 August 2015
Accepted: 27 September 2015
Published: 15 October 2015
In this study, we propose an ultra-facile approach to prepare a platinum silicide nanoparticle-modified tip apex (PSM tip) used for scanning Kelvin probe microscopy (SKPM). We combined a localized fluoride-assisted galvanic replacement reaction (LFAGRR) and atmospheric microwave annealing (AMA) to deposit a single platinum silicide nanoparticle with a diameter of 32 nm on the apex of a bare silicon tip of atomic force microscopy (AFM). The total process was completed in an ambient environment in less than 3 min. The improved potential resolution in the SKPM measurement was verified. Moreover, the resolution of the topography is comparable to that of a bare silicon tip. In addition, the negative charges found on the PSM tips suggest the possibility of exploring the use of current PSM tips to sense electric fields more precisely. The ultra-fast and cost-effective preparation of the PSM tips provides a new direction for the preparation of functional tips for scanning probe microscopy.
With the prosperous development of nanotechnology, the demand on nondestructive analysis of the distribution of charge density , magnetic field , surface potential , etc. is surging in nanometrology. In the field of nondestructive analysis, scanning Kelvin probe microscopy (SKPM) has been widely used to analyze the surface potential distribution of materials [4–6]. Spatial resolutions of the geometry and surface potential are both crucial issues in SKPM. Traditionally, apexes of silicon (Si) tips coated with metallic thin film, e.g., platinum-iridium alloy (PtIr), are widely used for SKPM. However, the spatial resolution was seriously limited because of the stray-field generated by the metallic coating [7–9]. To reduce this stray-field phenomenon, many nanostructures have been proposed for tip modifications, including carbon nanotube [10–12], Pt nanowire , single metallic nanoparticle (NP) [14, 15], etc. Moreover, for many decades, electron beam induced deposition (EBID) has been a major approach for tip modification [16–19]. However, the vacuum system required for the EBID process and the need to manipulate electron beams make the tip modification costly and inefficient. For these reasons, the development of nonvacuum technology for tip modifications has been presented. Electrodeposition  and electroless deposition  are both feasible approaches for tip modification under ambient conditions. Recently, we successfully prepared an apex of an Ag NP-modified silicon tip (Ag tip) by utilizing a localized fluoride-assisted galvanic replacement reaction (LFAGRR), which provides a facile and cost-effective process for tip modification . However, the instability of Ag under ambient conditions directly limits the commercialization of the Ag tips . In this paper, the LFAGRR was extended to prepare Pt NP-modified silicon tip apexes (Pt tips). Moreover, we introduced atmospheric microwave annealing (AMA) to further stabilize the tip apexes by transforming the Pt tips into platinum silicide NP-modified tip apexes (PSM tips). Scanning electron microscopy (SEM), transmission electron microscopy (TEM), SKPM, and electrostatic force microscopy (EFM) were employed to study the PSM tips and the corresponding Si-based Pt silicide NPs. Our results demonstrate that the PSM tips benefit from both high spatial resolutions of topography and surface potential. Moreover, the facile and cost-effective approach combining the LFAGRR and AMA provides a new direction for preparing functional tips for scanning probe microscopy.
Preparation of Pt and PSM Tips
Surface Morphology and Material Characterization
SEM (Hitachi S-4000) and TEM (JEOL JEM2010F) were employed to investigate the surface profile of the prepared samples. Energy-dispersive X-ray spectroscopy (EDS) was used to analyze the elemental composition. The SKPM and EFM images were acquired by a scanning probe microscope (Bruker D3100). The SKPM measurement parameters were image size = 2 μm, scanning rate = 0.2 Hz, lift height = 30 nm, Vac = (1.1–1.5) V, and ω2 = (31–35) kHz. The EFM measurement parameters were: image size = 1 μm, scanning rate = 0.5 Hz, lift height = 30 nm, and substrate bias = (0, −0.5, −1.0, −1.5) V, respectively. All measurements were performed in constant environment conditions with temperature = (20 ± 0.3) °C and relative humidity = (40 ± 5) % RH. All of the chemicals used in the experiment were reagent grade.
Results and Discussion
In summary, we proposed an ultra-facile process combining LFAGRR and AMA to prepare PSM tips under ambient conditions. The improved potential resolution of Si-based Ag nanoislands in SKPM measurement was realized. Moreover, the resolution of the topography was comparable to that of a bare silicon tip. In addition, the negative charges found on the PSM tips suggests the possibility of exploring the use of current PSM tips to sense electric fields more precisely. The ultra-fast and cost-effective preparation of the PSM tips provides a new direction for preparing functional tips for scanning probe microscopy.
The authors would like to express appreciation to the Ministry of Science and Technology (MOST) of the Republic of China, Taiwan, for the financial supports under the following contract numbers: MOST104-2221-E-492-001, MOST104-2623-E-492-001-ET, and NSC101-2112-M-492-002-MY3.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Hong J, Noh K, Park S-i, Kwun S, Khim Z (1998) Surface charge density and evolution of domain structure in triglycine sulfate determined by electrostatic-force microscopy. Phys Rev B 58(8):5078View ArticleGoogle Scholar
- Häberle T, Schmid-Lorch D, Karrai K, Reinhard F, Wrachtrup J (2013) High-dynamic-range imaging of nanoscale magnetic fields using optimal control of a single qubit. Phys Rev Lett 111(17):170801View ArticleGoogle Scholar
- Hallam T, Lee M, Zhao N, Nandhakumar I, Kemerink M, Heeney M et al (2009) Local charge trapping in conjugated polymers resolved by scanning Kelvin probe microscopy. Phys Rev Lett 103(25):256803View ArticleGoogle Scholar
- Nichols JA, Gundlach DJ, Jackson TN (2003) Potential imaging of pentacene organic thin-film transistors. Appl Phys Lett 83(12):2366–2368View ArticleGoogle Scholar
- Evers S, Senöz C, Rohwerder M (2013) Spatially resolved high sensitive measurement of hydrogen permeation by scanning Kelvin probe microscopy. Electrochim Acta 110:534–538View ArticleGoogle Scholar
- Hu Y, Berdunov N, Di CA, Nandhakumar I, Zhang F, Gao X et al (2014) Effect of molecular asymmetry on the charge transport physics of high mobility n-type molecular semiconductors investigated by scanning Kelvin probe microscopy. ACS Nano 8(7):6778–6787View ArticleGoogle Scholar
- Nonnenmacher M, O’Boyle MP, Wickramasinghe HK (1991) Kelvin probe force microscopy. Appl Phys Lett 58(25):2921–2923View ArticleGoogle Scholar
- Sacha GM, Verdaguer A, Martinez J, Saenz JJ, Ogletree DF, Salmeron M (2005) Effective tip radius in electrostatic force microscopy. Appl Phys Lett 86(12):123101–123103View ArticleGoogle Scholar
- Folks L, Best ME, Rice PM, Terris BD, Weller D, Chapman JN (2000) Perforated tips for high-resolution in-plane magnetic force microscopy. Appl Phys Lett 76(7):909–911View ArticleGoogle Scholar
- Minhua Z, Vaneet S, Haoyan W, Robert RB, Jeffrey AS, Fotios P et al (2008) Ultrasharp and high aspect ratio carbon nanotube atomic force microscopy probes for enhanced surface potential imaging. Nanotechnology 19(23):235704View ArticleGoogle Scholar
- Nguyen CV, Chao K-J, Stevens RM, Delzeit L, Cassell A, Han J et al (2001) Carbon nanotube tip probes: stability and lateral resolution in scanning probe microscopy and application to surface science in semiconductors. Nanotechnology 12(3):363View ArticleGoogle Scholar
- Hafner JH, Cheung C-L, Oosterkamp TH, Lieber CM (2001) High-yield assembly of individual single-walled carbon nanotube tips for scanning probe microscopies. J Phys Chem B 105(4):743–746View ArticleGoogle Scholar
- Chen PL, Su J, Shiao MH, Chang MN, Lee CH, Liu CW. Scanning electron beam induced deposition for conductive tip modification. Nano/Micro Engineered and Molecular Systems (NEMS), 2012 7th IEEE International Conference on; 2012 5–8 March 2012. doi:10.1109/NEMS.2012.6196836
- Lin C-T, Yu M-H, Su J, Chen P-L, Shiao M-H, Nemcsics A et al (2013) Localized electroless Ag plating at a tip apex for scanning Kelvin probe microscopy. Jpn J Appl Phys 52(6):06GF3–GF3-4Google Scholar
- Lin H-M, Chang M-N, Lin Y-S, Cheng C-C (2010) The manufacturing of a metallic nano-cluster at a tip apex for field-sensitive microscopy applications. J Nanosci Nanotechnol 10(7):4459–4464View ArticleGoogle Scholar
- Brown J, Kocher P, Ramanujan CS, Sharp DN, Torimitsu K, Ryan JF (2013) Electrically conducting, ultra-sharp, high aspect-ratio probes for AFM fabricated by electron-beam-induced deposition of platinum. Ultramicroscopy 133:62–66View ArticleGoogle Scholar
- Chen I-C, Chen L-H, Orme C, Quist A, Lal R, Jin S (2006) Fabrication of high-aspect-ratio carbon nanocone probes by electron beam induced deposition patterning. Nanotechnology 17(17):4322View ArticleGoogle Scholar
- Schiffmann KI (1993) Investigation of fabrication parameters for the electron-beam-induced deposition of contamination tips used in atomic force microscopy. Nanotechnology 4(3):163View ArticleGoogle Scholar
- Utke I, Hoffmann P, Berger R, Scandella L (2002) High-resolution magnetic Co supertips grown by a focused electron beam. Appl Phys Lett 80(25):4792–4794View ArticleGoogle Scholar
- Elechiguerra JL, Larios-Lopez L, Liu C, Garcia-Gutierrez D, Camacho-Bragado A, Yacaman MJ (2005) Corrosion at the nanoscale: the case of silver nanowires and nanoparticles. Chem Mater 17(24):6042–6052View ArticleGoogle Scholar
- Ye W, Liu J, Liu Q, Zhou F, Liu W (2010) Surfactant-free and controllable synthesis of hierarchical platinum nanostructures and their comparative studies in electrocatalysis, surface-enhanced Raman scattering and surface wettability. Electrochim Acta 55(28):8649–8654View ArticleGoogle Scholar
- Bykov YV, Eremeev AG, Zharova NA, Plotnikov IV, Rybakov KI, Drozdov MN et al (2003) Diffusion processes in semiconductor structures during microwave annealing. Radiophys Quantum El 46(8–9):749–755View ArticleGoogle Scholar
- Yao-Jen L, Bo-An T, Chiung-Hui L, Zheng-Yao C, Fu-Kuo H, Po-Jung S et al (2013) Low-temperature microwave annealing for MOSFETs with high-k/metal gate stacks. IEEE Electron Device Lett 34(10):1286–1288View ArticleGoogle Scholar
- Bhaskaran H, Sebastian A, Despont M (2009) Nanoscale PtSi tips for conducting probe technologies. IEEE Trans Nanotechnol 8(1):128–131View ArticleGoogle Scholar
- Bhushan B, Palacio M, Kwak KJ (2008) Thermally-treated Pt-coated silicon AFM tips for wear resistance in ferroelectric data storage. Acta Mater 56(16):4233–4241View ArticleGoogle Scholar
- Chou TC (1991) High temperature reactions between SiC and platinum. J Mater Sci 26(5):1412–1420View ArticleGoogle Scholar
- Takahashi Y, Ishii H, Murota J (1985) New platinum silicide formation method using reaction between platinum and silane. J Appl Phys 58(8):3190–3194View ArticleGoogle Scholar
- Wang D, Penner S, Su DS, Rupprechter G, Hayek K, Schlögl R (2003) Silicide formation on a Pt/SiO2 model catalyst studied by TEM, EELS, and EDXS. J Catal 219(2):434–441View ArticleGoogle Scholar
- Liu G, Yang K, Li J, Tang W, Xu J, Liu H et al (2014) Surface diffusion of Pt clusters in/on SiO2 matrix at elevated temperatures and their improved catalytic activities in benzene oxidation. J Phys Chem C 118(39):22719–22729View ArticleGoogle Scholar
- Murarka SP (1983) Silicides for VLSI applications. Academic Press; San Diego. ISBN:978-0-12-511220-8. doi:10.1016/B978-0-08-057056-3.50001-X
- Murarka S, Kinsbron E, Fraser D, Andrews J, Lloyd E (1983) High temperature stability of PtSi formed by reaction of metal with silicon or by cosputtering. J Appl Phys 54(12):6943–6951View ArticleGoogle Scholar